[CONTRIBUTION FROM THE JOHN HARRISON LABORATORY s o . 52.1
SEPARATION OF TUNGSTEN TRIOXIDE MOLYBDENUI7 TRIOXIDE.
nv MAX J . R ~ E G E S B E RAGN D EDGAR F. S M I T H Received Scptemher :,
HE separation of tungsten from molybdenum is always of
interest to those who are brought in contact with analytical methods. It has been the subject of numerous investigations and much discussion, and while comparatively good methods exist for this purpose, the analyst continues to seek for others, hoping that eventually he shall find a procedure which will be satisfactory in all respects and under nearly all conditions. T h e writers have not discovered the method p a r excellence, but desire to offer briefly, in the following lines, their experience in pursuing a suggestion made in an article emanating from this insoluble in concentralaboratory ; viz., ‘ ‘ tungstic acid is ted or dilute sulphuric acid, hot or cold, whereas molybdenum trioxide is very easily and rapidly dissolved, so that we have in this deportment a very simple and exact method for the separation of the two metals.”’ No analytical data accompanied this declaration ; therefore it seemed not improper to attempt to learn the conditions most favorable for the separation. Upon trial it was found that sulphuric acid of specific gravity I .378, dissolved molybdenum trioxide very readily and apparently did not affect the tungsten trioxide. Acid of this concentration was, therefore, used with the following mixture of the two oxides : I. 0 . 7 3 j j gram of tungsten trioxide and 0.0185 gram of molybdenum trioxide were digested for a few minutes with Z j cc. of warm sulphuric acid. T h e insoluble portion was filtered out and washed with water containing sulphuric acid. After drying it was ignited and weighed. I t equaled 0.7350 gram. T h e other trials, conducted in precisely the same manner, were a s follows :
. . ..
Tungsten trioxide t a k e n . . . . 1.0638 Molybdenum trioxide taken 2.2712 Tungsten trioxide found . 1.0630
En. D. Desi : This Journal, 19,
0.8868 1.1986 0.8866
0.5996 1.0770 0.5996
T h e filtrate containing the dissolved molybdic acid showed no tungstic acid upon examin at'ion. These results indicate that where the two oxides are present together this mode of separation is apparently of value and merits consideration. A weighed quantity of a ferric salt equivalent to 5 grams of ferric hydroxide was precipitated with ammonia water and theresulting precipitate, after being mashed, was mixed in a beaker with different amounts of tungsten trioxide, and the resulting mixture was then digested with sulphuric acid of the strength of that used in the preceding experiments. T h e residual oxide was treated as before : Tungsten trioxide taken Ferric hydroxide taken . Tungsten trioxide found
1. 11. 111. IV. V. VI. G r a m s . G r a m s . G r a m s . Grains. G r a m s . Grams. 0.5282 0.2087 1.3270 0.2004 o.go91 0.2263
.. .. 5.0000 . . 0.j278
I ,3265 0.2003
W e may conclude from these trials that the solubility of the trioxide in the sulphuric acid is in no wise affected by the presence of the iron. UNIVERSITY OF P E N N S T L V A S I A .
NEW BOOKS. THE MINERALINDUSTRY : ITS STATISTICS, TECHNOLOGY, AXD TRADE IN THE UXITED STATESA N D OTHER COUNTRIES, TO THE ENDOF 1899. EDITEDBY RICHARD P. ROTHWELI,. Vol. VIII. Large Svo. xxviii+g86 pp. With many illustrations. New Y o r k : The Scientific Publishing Co. Price, $5.00.
This new annual voluine of a well-known and greatly valued series fully sustains the reputation already obtained. T h e difficulty in obtaining accurate information of this character is well known, and the rapid publication of a large volume like this, requiring the cooperation of so many persons, reflects the greatest credit upon all those concerned in it. T h e year 1899 was a great year for the mineral industry in the United States, the production in nearly all metals and minerah showing a decided increase. This is especially noticeable in Portland cement, where the increase is from 3,584,586 barrels of 400 lbs. in 1898 to 5,805,620 barrels in 1899. Among the new products listed in recent years are fcrroniolybdenum, 6,000 lbs. in 1899 ; molybde25-22